Norma ASTM A570 - 1979...
By Authority Of THE UNITED STATES OF AMERICA
Legally Binding Document By the Authority Vested By Part 5 of the United States Code § 552(a) and Part 1 of the Code of Regulations § 51 the attached document has been duly INCORPORATED BY REFERENCE and shall be considered legally binding upon all citizens and residents of the United States of America. HEED THIS NOTICE: Criminal penalties may apply for noncompliance.
e Document Name: ASTM A570: Hot-Rolled Carbon Steel Sheet and Strip, Structural Quality
24 CFR 200, Subpart S
American Society for Testing and Materials
Official Incorporator: THE EXECUTIVE DIRECTOR
OFFICE OF THE FEDERAL REGISTER WASHINGTON, D.C.
~~l~ =RJ~~~~t:J ANSljASTMA 570 - 79
Standard Specification for
HOT-.ROLLED CARBON STEEL SHEET AND STRIP, STRUCTURAL QUALlTY1 This Standard is issued under the fixed designation A 570; the number immediately following the designation indicates the year of original adoption or, in the case-of revision,. the year oflast revision. A number in parenthese_s indicates the year of last reapproval. This specification has been approved for use by agencies of the Department of Defonse and for listing in the DoD Index of Specifications and Standards. -
1. Scope 1.1 This specification covers hot-rolled carbon steel sheet and strip of structural quality in cut lengths or coils. This material is intended for structural pUI:poses where mechanical test values are required, and is avail" able in a maximum thickness of 0.2299 in. (5.8 mm) except as limited by Specification A 568. 1.1.2 The following grades are covered in this specification: Mechanical Properties Grade 30 33
36 40 45 50
Yield Point, min, psi (MPa) 30 000 (2\0) 33 000 (230) 36 000 (250) 40 000 (280) 45 000 (3\0) 50 000 (340)
Tensile Strength, min, psi (MPa) 49 000 (340) 52 000 (360) 53 000 (365) 55 000 (380)· 60 000 (4\0) 65 000 (450)
I-The values stated in inch-pound units are to be regarded as the standard.· NOTE
2. Applicable Documents 2.1 ASTM Standard: A 568, Specification for Steel, Carbon arid High-Strength Low-Alloy Hot~Rolled Sheet, Hot-Rolled Strip, and ColdRolled Sheet, General Requirements 2 3. General Requirements for Delivery 3.1 Material furnished under this specification shall conform to the applicable requirements of the current edition of Specification A 568, unless otherwise provided herein. 4. Ordering Information 4.1 Orders for material under this specifi-
cation shall include the following information, as required, to describe the required material adequately: -, 4.1.1 ASTM specifieation number and date of issue, and grade, 4.1.2 Copper-bearing steel (if required), 4.1.3 Special requirements (if required), 4.1.4 Name of material (hot~rolied sheets or strip), 4.1.5 Condition (Material t6 this specification is furnished in the hot-rolled condition. Pickled (or blast cleaned) should be specified if required. Material so ordered will be oiled unless ordered dry), . 4.1.6 Dimensions, including type of edges, 4.1.7 Coil size requirements, and 4.1.8 Cast or heat (formerly ladle) analysis or test report (request, ifrequired). NOTE 2 - A typical ordering description is as follows: ASTM A 570, Grade 36, Hot-Rolled Sheets, 0.075 by 36 cut edge by 96 in.
S. Chemical Requirements 5.1 The cast or heat analysis of the steel shall conform to the requirements prescribed in Table 1. 6. Physical Requirements
6.1 Tensile Properties-The material as
1 This specification is under the jurisdiction .of ASTM Committee A-l on Steel, Stainless Steel and Related Alloys, and, is the direct responsibility of Subcommittee A01.l9 oil Sheet Steel and Steel Sheets. Current edition approved Aug. 31, 1979. Published October 1979. Originally published as A 570 - 66 T. Last previous edition A 570 - 78. 2 Annual Book of ASTM Standards, Part 3.
finished material from a heat or lot is less than 50 tons, only one tension test and one bend test shall be made. When material rolled from one heat differs 0.050 in. (1.27 mm) or more in thickness, one tension test and one bend test shall be made from both the thickest and thinnest material rolled regardless of the weight represented. 8.2 Retests - If one test fails, two more tests shall be run from the same lot, in which case both tests shall conform to the requirements prescribed in this specification; otherwise, the lot under test shall stand rejected.
represented by the test specimens shall conform to the requirements as to tensile properties prescribed in Table 2. 6.2 Bending Properties- The bend test specimens shall stand being bent at room temperature in any direction through 180 deg without cracking on the outside of the bent portion to an inside diameter which shall have a relation to the thickness of the specimen as prescribed in Table 3. 7. Test Specimens 7.1 Tension test specimens shall be taken longitudinally.
9. Packaging 9.1 Coil Size - Small coils result from the cutting of full-size coils for center test purposes. These small coils are acceptable under this specification.
8. Number of Tests 8.1 Two tension tests and two bend tests shall be made from each heat or from each lot of 50 tons (45 Mg). When the amount of TABLE 1
Chemical Requirements Composition, %
Grades 30, Grades 45 33, 36, and 40 and 50
Carbon, max Manganese, max Phosphorus, max Sulfur, max Copper, when copper is specified, min
0.25 0.90 0.04 0.05
1.35 0.04 0.05 0.20
TABLE 2 Tensile Requirements Grade 36
49 000 (340)
52 000 (360)
53 000 (365)
55 000 (380)
60 000 (410)
65 000 (450)
30 000 (210)
33 000 (230)
36 000 (250)
40 000 (280)
45 000 (310)
50 000 (340)
Grade 30 Tensile strength, min, psi (MPa) Yield point, min, psi (MPa) Elongation in 2 in. (50 mm), min, %, for thicknesses: 0.2299 to 0.0972 in. (5.84 to 2.46 mm), inel 0.0971 to 0.0636 in. (2.45 to 1.62 mm), inel 0.0635 to 0.0255 in. (1.61 to 0.65 mm), incl Elongation in 8 in. (200 mm), min, %, for thicknesses: 0.2299 to 0.0972 in. (5.84 to 2.46 mm), inel 0.0971 to 0.0892 in. (2.45 to 2.26 mm), inel
TABLE 3 Bend Test Requirements Grade
Ratio of Bend Diameter to Thickness of Specimen
30 33 36 40 45 50
1>'. 2 21'2 3
The American Society for Testing and Materials takes no position respecting the validity of any patent rights asserted in connection with any item mentionetf in this standard. Users oJ this stantfard are expressly aavised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own resppnsibility. This standard is subject to revision at any time by the responsible technical committee and must 'be reviewed every five years and if not revised, either reapproved or withdrawn. Your comments are invited either for reviston of this standard or for additional standards and should be addressed to ASTM Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair 'hearing you should make your views known to the ASTM Committee on Standards, 1916 Race St., Philadelphia, Pa. 19103, which 'will schedule a further hearing ,regarding your comments. Failing satisfaction there, you may appeal to the ASTM Board of Directors.